. Angewandte Minireviews

S. V. Krivovichev

DOI: 10.1002/anie.201304374

Inorganic Crystal Structures

Which Inorganic Structures are the Most Complex? Sergey V. Krivovichev* crystallography · information theory · inorganic structures · structural complexity · structural elucidation

The discovery of the diffraction of X-rays on crystals opened up a new era in our understanding of nature, leading to a multitude of striking discoveries about the structures and functions of matter on the atomic and molecular scales. Over the last hundred years, about 150 000 of inorganic crystal structures have been elucidated and visualized. The advent of new technologies, such as area detectors and synchrotron radiation, led to the solution of structures of unprecedented complexity. However, the very notion of structural complexity of crystals still lacks an unambiguous quantitative definition. In this Minireview we use information theory to characterize complexity of inorganic structures in terms of their information content.

1. Introduction The evolution of matter towards states of higher complexity in the course of the evolution of the Universe is one of the most interesting topics in modern science and in modern chemistry in particular.[1] A number of different approaches exist that allow the complexity of chemical, biological, technological, and even social systems to be quantitatively evaluated.[2] Most of these approaches are based upon the extensive use of concepts and techniques borrowed from the information theory developed in the second half of the 20th century as a theory of communication and transmission of information.[3] Nowadays complexity theory is a well-developed field of computer science with interdisciplinary applications in many areas of theoretical and applied sciences.[4] It is interesting, however, that complexity theorists have always regarded crystals as “intuitively simple objects”,[5] in contrast to much more complex and dynamic biological systems. On the other hand, it was largely appreciated that crystal structures may possess different degrees of complexity, which has been reflected in the titles of scientific papers with the use of expressions such as “complicated structure”, “the most complex structure”, “complexity”, “complex superstructures”, “a masterpiece of structural complexity”.[6] However, until recently, the complexity of crystal structures was

[*] Prof. Dr. S. V. Krivovichev Department of Crystallography, St. Petersburg State University University Emb. 7/9, 199034 St. Petersburg (Russia) E-mail: [email protected]

654

destined to be “largely a qualitative, frequently intuitive, notion”,[7] which escaped a quantitative definition. Perhaps, the first attempt to evaluate structural complexity of crystals should be assigned to the Linus Paulings fifth (“parsimony”) rule “determining the structure of complex ionic crystals”:[8] “the number of different types of constituents in a crystal tends to be small.” Hawthorne[9] noted that “this rule has not seen much use, apart from in teaching, but it certainly seems to hold reasonably well, and its underlying cause is certainly of interest.” The certain advantage of crystals is that their almost infinite network of atoms and bonds can be described by a rather small volume of space called the elementary unit cell. Of even smaller volume is the asymmetric unit, which only contains symmetrically inequivalent atoms. To provide a quantitative definition of crystal-structure complexity, Baur et al.[10] suggested to use topological and crystallographic parsimony indices, It and Ic, defined by Equations (1) and (2), I t ¼ ðteÞ=t

ð1Þ

I c ¼ ðceÞ=c

ð2Þ

where e is the number of different chemical elements, and t and c are the numbers of topologically and crystallographically distinct atom sites in the asymmetric unit, respectively. Baur et al.[10] pointed out that the topological parsimony index is of primary importance and suggested subdividing structures into lavish (It > 0.66), intermediate (0.66 > It > 0.33), and parsimonius (It < 0.33). Both indices are not sensitive either to chemical complexity or symmetry and reflect only relations between the number of chemical elements and the number of topologically or crystallographically distinct atom sites.

2014 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim

Angew. Chem. Int. Ed. 2014, 53, 654 – 661

Angewandte

Chemie

Inorganic Crystal Structures

An alternative approach to structural complexity was suggested by Lister et al.,[6b,c] who used the number of atoms in the asymmetric unit as a measure of complexity for a commensurate structure. This method has many advantages but, unfortunately, does not provide an appropriate quantification of the complexity of high-symmetry structures, such as, paulingite, a complex natural zeolite, which was identified by Mackay and Klinowski[11] as one of the most complex inorganic structure. Mackay[12] and later Estevez-Rams and Gonzlez-Frez[13] proposed to estimate the complexity of crystal structures on the basis of the complexity of algorithms that can be used to generate them from an unordered array of atoms. This concept is of great interest, but, in its present state, requires a high level of abstraction and imagination and cannot be applied to crystal structures in an easy and unambiguous way. In this Minireview, a different method is employed to evaluate the complexity of structures, which is based upon the relatively simple application of Shannon information theory and allows both size- and symmetry-dependent properties of complex structures to be quantitatively evaluated, thus combining their symbolic and combinatorial complexities[14] in the same measure.

2. Basic Concepts In the framework of classical information theory, information content H of a message M consisting of v symbols that belong to the k equivalence classes is calculated according to the following Shannon formula [Eq. (3)] H¼

k X

pi log2 pi ½bits=symbol

ð3Þ

i¼1

subdivided into equivalence classes according to their crystallographic orbits, that is, two atoms belong to the same class if they are symmetrically equivalent. This led to the following formula to calculate the structural information content, IG, of a crystal structure [Eq. (5)] IG ¼

k X

where k is the number of crystallographic orbits and pi is the probability of occurrence of the atom of the ith crystallographic orbit [Eq. (6)] pi ¼ mi =v

ð6Þ

where mi is the multiplicity of the crystallographic orbit relative to the reduced unit cell, and v is the number of atoms in the reduced unit-cell. For instance, the structure of lopezite, K2Cr2O7,[17] is triclinic, space group P1¯. All the atoms in the structure occupy 2i Wyckoff sites: there are four K, four Cr, and fourteen O sites, which corresponds to the total number of 22 equivalence classes. The total number of atoms in the reduced unit cell (which in this case coincides with the crystallographic unit cell) is 44. Atoms from each equivalence class has the same probability of occurrence, which is equal to 2/44 = 0.0455. The structural information content for lopezite is given by Equation (7). I G ¼ 22 ð2=44Þ log2 2=44 ¼ 4:459 bits=atom

pi ¼ mi =v

ð4Þ

where mi is the number of symbols in M that belong to the ith equivalence class. Following theoretical works on the topological complexity of graphs and networks,[2b, 15] Krivovichev[16] proposed to consider the reduced elementary unit cell of a crystal structure as a message consisting of v atoms. The atoms are

Sergey Krivovichev received his Ph.D. (1997) and D.Sc. (2002) degrees from St. Petersburg State University and carried our post-doctoral research in the U.S., Germany, Switzerland, and Austria. Since 2005, he is a Full Professor and Chairman of Department of Crystallography, St. Petersburg State University. His research interests include inorganic structural chemistry, mineralogy, crystallography, nuclear materials, and applications of complexity theory to natural and artificial objects.

Angew. Chem. Int. Ed. 2014, 53, 654 – 661

ð7Þ

The total information content of a crystal structure is determined by the Equation (8). I G,total ¼ v I G ðbits=unit-cellÞ

where pi is the probability of occurrence of the ith symbol [Eq. (4)]:

ð5Þ

pi log2 pi ½bits=atom

i¼1

ð8Þ

For lopezite, IG,total = 44 4.459 = 196.196 bits per unit-cell (bits/u.c.). The maximal structural information content, IG,max, for a crystal structure with v atoms occurs, where all atoms are non-equivalent according to the corresponding space group. It can be calculated as Equation (9). I G,max ¼ log2 v ðbits=atomÞ

ð9Þ

For IG to be independent of v, we may define the normalized structural information content, IG,norm, as Equation (10). I G,norm ¼ I G =I G,max ¼ ½

k X

pi log2 pi =log2 v

ð10Þ

i¼1

For the structure of lopezite, IG,max = log2 44 = 5.459 bits/atom and IG,norm = 4.459/5.459 = 0.817. Note that IG,norm is a dimensionless quantity in the range from 0 to 1. The information-based complexity measures allow us to introduce the concept of information density, which can be defined as a number of bits of information per cubic ngstrçm [Eq (11)].

2014 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim

www.angewandte.org

655

. Angewandte Minireviews 1inf ¼ I G,total =V ðbits 3 Þ

S. V. Krivovichev

ð11Þ

BaTiO3 is more complex than rutile, TiO2 (rutile), whereas rutile is more complex than NaCl (halite). Both parsimony For lopezite, 1inf = 0.270 bits 3. For another modification of indices, It and Ic,[10] cannot discriminate between the complex[18] 3 K2Cr2O7, 1inf = 0.156 bits , which indicates its lower ities of the three structures, whereas the number of atoms complexity compared to lopezite. It is important that within the asymmetric unit (c)[6b,c] cannot distinguish between information density should be calculated using the volume the complexities of tetragonal rutile and cubic halite. On the of the reduced unit cell. other hand, ranking of the structures according to the IG,total For two structures with similar unit cells but different values is in agreement with the intuitive feelings (in bits per symmetry, information density will be higher for the structure unit cell): 6.855 (BaTiO3) > 5.510 (rutile) > 2.000 (halite). In with lower symmetry (and higher complexity). For instance, general, it may be concluded that the parsimony indices[10] do cation ordering within the same unit cell would lead to the not possess enough discriminative power, whereas the c formation of a superstructure with higher information density parameter underestimates complexities of highly symmetrical than that of the original structure. This situation shows that structures and structures with non-general orbits. unit-cell volume alone cannot be considered as a measure of Since total information content of the crystal structure, structural complexity, since it reflects only the symbolic IG,total, is defined per unit cell, it is possible to calculate a total complexity of the system and is not sensitive to its combinainformation amount of a particular crystal. For instance, torial complexity. a 1 mole crystal of a-quartz, space group P3221, Z = 3, Information density can also be used as a measure of contains approximately 2.00738 1023 unit cells calculated as complexity for the crystal structures of solids with similar the Avogadro number, 6.02214 1023,[21] divided by Z = 3. The composition. The fact that complexity is a function of both total information content of the crystal structure of a-quartz is information content and unit-cell volume makes it dependent IG,total = 8.265 bits/u.c. Therefore, the total information conupon the size of atoms and ions that make up the respective tent of the 1 mole quartz crystal is equal to approximately crystal, as well as upon temperature and pressure. Suanite, 16.59100 1023 bits. It should be emphasized that, clearly, [19] [20] Mg2B2O5, and natrosilite, Na2Si2O5, have the same total structural information of a crystal consisting of billions of unit cells is redundant or algorithmically compressible.[12] Neverstructural information content (114.117 bits/u.c.), but their information densities are drastically different (0.333 and theless, the full amount of this (redundant) information can 0.242 bits 3, respectively), which is a consequence of the be calculated from the amount of the respective crystalline substance expressed either in molar, mass, or volumnar different ionic radii of the Mg2+ and Na+ ions, on the one quantities. This means that, similar to mass, entropy, volume, hand, and of the B3+ and Si4+ ions, on the other. However, for example, information is an “extensive” property as while information density cannot be used to compare opposed to the “intensive” properties such as temperature structures with different chemical compositions, it is a useful and pressure. parameter for the investigation of behavior of structural To explain this point further, consider the following information in the course of phase transitions induced by sequences: a) 010101010101010101, b) 101001101001101001, temperature and pressure, that is, when chemical composition and c) 010001111000101101. To store these sequences, any is a constant parameter. computer would need exactly 18 bits for each, which means Table 1 presents comparison of the values of the complexthat the amount of information expressed in bits is identical ity parameters defined according to Baur et al.,[10] Lister for the three sequences. However, the sequence (c) cannot be et al.,[6b,c] and this work, applied to different simple and compressed, whereas the sequences (a) and (b) are algorithcomplex inorganic structures. These data indicate certain mically compressible: the sequence (a) can be represented as advantages in the use of information-based complexity “repeat 01 nine times”, whereas (b) as “repeat 101001 three parameters (and, in particular, the IG,total parameter) as times”. By analogy, crystals can be constructed by repeating compared to the purely crystallographic parameters (v, c, It, its unit cell in a three-dimensional space; however, its full and Ic). For instance, according to the intuitive feelings, information content will be a function of the number of these repeats, just as the full information content Table 1: Comparison of the values of different complexity parameters for the same inorganic crystal of the sequence (b) is the function structures of the number of repeats of the Structure ICSD v c It[c] Ic[d] IG IG,total IG,norm sequence “101001”. It can be ar[a] [b] code [atoms] [atoms] [bits] [bits/u.c.] gued that, in the framework of this NaCl 53815 2 2 0 0 1.000 2.000 1.000 approach, a piece of glass would 53997 6 2 0 0 0.918 5.510 0.355 TiO2 rutile contain more information than the BaTiO3 cubic 56093 5 3 0 0 1.371 6.855 0.590 crystal with the corresponding com36261 24 7 0 0.71 2.752 66.039 0.600 SiO2 coesite Ba2Ti9O20 35711 124 62 0.90 0.95 5.954 738.320 0.856 position, since, because of the abBa6Ti17O40 49576 126 34 0.89 0.91 5.057 637.137 0.725 sence of the long-range order, the SiP2O7 cubic 66861 1080 50 0 0.94 5.570 6015.280 0.553 structure of the glass is unique in Cu2Li2P6O18 2149 56 28 0.73 0.86 4.807 269.212 0.828 each point of the piece. However, [a] Number of atoms per reduced unit cell. [b] Number of atoms per asymmetric unit.[6b,c] [c] Topological this information is meaningless, since local distortion of the strucparsimony index.[10] [d] Crystallographic parsimony index.[10]

656

www.angewandte.org

2014 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim

Angew. Chem. Int. Ed. 2014, 53, 654 – 661

Angewandte

Chemie

Inorganic Crystal Structures

ture of the glass would not alter its properties. The IG value proposed above measures structural information per atom, whereas the IG,total value defines information amount per smallest unit, which forms the whole structure by its repeating in three dimensions. As can be seen from Table 1, the most adequate parameter to evaluate complexity of a crystal structure is IG,total.

3. Complexity of Inorganic Structures: Statistics To analyze the complexity of inorganic structures on a large-scale basis, complexity parameters have been calculated for all the crystal-structure entries stored in the Inorganic Crystal Structure Database (ICSD)[22] using the TOPOS program package.[23] Figure 1 shows distribution of

Figure 2. Diagrams showing relations between complexity parameters for the ICSD reports: number of atoms per unit cell (v), structural information content per atom (IG) and per unit cell (IG,total): point diagram (a); each point corresponds to a single ICSD report (two reports with IG,total > 35 000 bits are omitted for clarity) and a contour map (b) colors show the range of the IG,total values).

Figure 1. Histogram showing distribution of inorganic crystal-structure reports stored in the Inorganic Crystal Structure Database (ICSD) according to the values of the information-based IG and IG,total parameters.

the ICSD reports according to the information contents per atom (IG) and per unit-cell (IG,total). According to the IG,total values, all structures can be subdivided into very simple, simple, intermediate, complex, and very complex (Table 2). It can be seen from Figure 1 that most ICSD entries are for very simple and simple structures that together constitute about 75 % of the ICSD data. This reflects the fact that structurally and chemically simple inorganic compounds have been most studied over the last hundred years, though the general current trend is towards the elucidation of structures with increasing complexity (see below).

Table 2: Classification of inorganic crystal structures according to their complexity (information content per unit cell). Category

IG,total [bits/u.c.]

Number of ICSD entries

very simple simple intermediate complex very complex

< 20 20–100 100–500 500–1000 > 1000

ca. 55 000 ca. 50 000 ca. 33 000 ca. 5000 ca. 3000

Angew. Chem. Int. Ed. 2014, 53, 654 – 661

Figure 2 shows relations between the information contents per atom (IG) and per unit-cell (IG,total), and the number of atoms in the unit cell (v) (note that all the quantities are referred to the reduced unit cells). It can be seen that there is a general positive correlation between v and IG,total. However, structures with the same number of atoms per unit cell may differ in their IG,total values by several hundreds of bits, which shows that, in agreement with the previous conclusion, the purely crystallographic v parameter cannot be used as a single complexity measure, since it accounts for the size of the structure only, and not for its symmetry. The symmetrysensitive parameter is IG, and the IG,total parameter provides combination of both size- and symmetry-sensitive complexity measures.

4. Most Complex Inorganic Structures Analysis of the 2000 most-complex structures stored in the ICSD according to their belonging to specific classes of inorganic compounds is shown in Figure 3. About 90 % of all these compounds are structures based upon nanoscale-sized clusters with 82 % represented by Mo-, W-, and V-based polyoxometallates. Among other classes are: oxides and oxysalts (e.g., silicates, sulfates, borates), zeolites and microporous framework materials, intermetallic compounds, borides and silicides, superstructures of simpler structure types, sulfides and selenides, and halogenides. The most complex inorganic structure reported to date is that of the intermetallic compound Al55.4Cu5.4Ta39.1 (ACT-

2014 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim

www.angewandte.org

657

. Angewandte Minireviews

S. V. Krivovichev

Figure 3. Classification of the 2000 most-complex inorganic structures according to their chemical identity: 1) Mo-, W-, V-based polyoxometallates; 2) oxides and oxysalts; 3) structures containing (nano)clusters; 4) zeolites and microporous framework compounds; 5) intermetallic compounds (including borides and silicides); 6) fullerene-based structures; 7) uranyl peroxide nanospheres; 8) superstructures of simple structure types; 9) Nb-, Ti-based polyoxometallates; 10) sulfides and selenides; 11) halogenides.

71).[24] Its total structural information content is equal to 48 538.637 bits/u.c. The reduced unit cell contains v = 5814 atom sites and the structural information content per atom (IG) is 8.349 bits. The exceptional complexity of this structure is the result of the combination of different structural modules, which was described by Steurer and coworkers[24] as follows: The Al12Ta28 fullerene cluster shells (orange polyhedra in Figure 4 a consisting of 40 faces and 76 vertices) are linked by the Ta15 bifrusta (red polyhedra consisting of 12 faces and 15 vertices) into a porous framework with large cavities occupied by supertetrahedral clusters of two types. The first type (Figure 4 b,c) consists of 146 Tacentered Al12 Friauf polyhedra, Ta8 hexagonal bipyramids, and Al12Ta28 fullerene shells. The second type is formed by ten Al102Ta57 fullerenes (Figure 4 e). The supertetrahedral clusters

Figure 4. Structural building principle of Al55.4Cu5.4Ta39.1 (ACT-71). Reproduced with permission from Ref. [24].

658

www.angewandte.org

form two interpenetrating diamond-type networks (Figure 4 d) and, together with the fullerene–bifrustum framework (Figure 4 a), form the unit cell of extraordinary complexity (Figure 4 f). The second most complex structure is that of (C(NH2)3)136[{(C(NH2)3)20(H2O)100}{(Mo)Mo5O21(H2O)6}12{Mo2O4(H2PO2)}20{Mo2O4(SO4)}10][{(C(NH2)3)20(H2O)80} {(Mo)Mo5O21(H2O)6}12{Mo2O4(H2PO2)}12{Mo2O4(SO4)}18](H2O)400,[25] which contains spherical polyoxomolybdate cluster of the type {(Mo)Mo5}12(spacer)30 (one of the “Keplerates”)[26] (Figure 5 a,b). The nanocavity inside the cluster is occupied by the (H2O)100 nanodrop of water with H2O

Figure 5. Polyoxometalates nanoscale clusters from selected very complex inorganic structures (skeletal representation is given for each cluster showing the topology of the metal-O-metal links): a,b) “Keplerate” cluster from the structure of {[(NH2)3C]52}{(Mo)Mo5O21(H2O)6}12 {Mo2O4(SO4)}10{Mo2O4(H2PO2)}20 (pink and red polyhedra are Mo and P coordination polyhedra, respectively); c,d) uranyl peroxide nanosphere with the C50 fullerene topology (yellow polyhedra are uranyl hexagonal bipyramids); e,f) 18-nuclear Ti-Nb-polyoxometalate cluster from the structure of [N(CH3)4]20[Ti12Nb6O44]2(H2O)73 (Ti and Nb polyhedra are shown as blue and green, respectively).

molecules arranged in three concentric shells. The enormous complexity (IG,total = 45341.050 bits/u.c., v = 5128 atoms/u.c.) is not only due to the size of the clusters, but also due to the fact that there are two crystallographically independent clusters in the structure with 3¯m and 2/m site symmetries. Very complex structures with giant clusters are dominated by Mo-, W-, and V-polyoxometallates. However, oxo-nanoclusters of other metals can also assemble to form structures of high complexity. A prominent example is the uranyl peroxide nanospheres formed by linkage of uranyl ions, UO22+, through peroxide groups (Figure 5 c,d).[27] The maximal number of uranyl ions in such clusters prepared to date is 120, and some of the clusters adopt fullerene topologies.[28] It is noteworthy that uranyl peroxide nanospheres are porous and their cavities may accommodate various cations and H2O molecules. Figure 5 e shows the [Ti12Nb6O44]10 cluster from the structure of [N(CH3)4]20[Ti12Nb6O44]2(H2O)73.[29] Despite the obvious high symmetry of the cluster (m3¯m) that can be appreciated from its skeletal representation (Figure 5 f), the symmetry of the crystal structure is monoclinic (space group P21/c).

2014 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim

Angew. Chem. Int. Ed. 2014, 53, 654 – 661

Angewandte

Chemie

Inorganic Crystal Structures

Figure 6. The nanoscale-domain superstructure of Nd7/12Li1/4TiO3 consisting of square-shaped Li-rich regions (white) separated by zigzagging boundary regions of a Nd-rich structure (orange).

Another complexity-generating mechanism in inorganic materials is formation of superstructures either by atomic ordering or displacive phase transitions. Figure 6 shows an ordered nano-checkerboard superlattice observed in the structure of Nd7/12Li1/4TiO3 by transmission electron microscopy and modeled by Rietveld refinement.[30] The structure in general belongs to the perovskite structure type (ABO3) with Ti in the B site and Li and Nd in the A site. The Li–Nd ordering results in formation of square-shaped nanoscale domains of a Li-rich phase separated by a zig-zagging boundary region consisting of a Nd-rich phase.[30] The resulting supercell has the dimensions 14ap 28ap 2ap, where ap is the unit-cell parameter of a simple perovskite. The total information content of the structure equals to 16 634.804 bits/ u.c. with v = 1973 atoms/u.c. An example of a very complex structure with complexity generated by displacive phase transitions on cooling is that of [Mo2P4O15] which can be written as [(MoO)2P4O13].[6b,c] The structure consists of corner-sharing MoO6 octahedra interlinked by linear P4O13 tetramers of tetrahedra. Its topological complexity (i.e., complexity of an archetype framework) is rather small (IG,total = 144.477 bits/u.c.),[31] whereas real structures are very complex (7748.048 bits/u.c. for monoclinic 120 K a-phase and 4022.549 bits/u.c. for triclinic 573 K bphase).[6b,c] The high complexity of the real structures compared to the much simpler archetype is due to the local bonding requirements that led to the formation of extended superstructures. This example is remarkable in that the symmetry of a high-temperature b-phase (space group P1¯) is lower than the symmetry of a low-temperature a-phase (space group Pn). However, the information amount of the high-temperature phase is smaller than that of the lowtemperature phase, which shows that, at least in this case, the information amount decreases with the increasing temperature, despite the decreasing symmetry. The high topological and structural complexity of zeolites and microporous oxide-based frameworks has long been recognized. One of the most complex zeolites[16c] and the most complex mineral known to date[16d] is paulingite, K6Ca16(Al38Si130O336)(H2O)113,[32] with IG,total = 6766.998 bits/ u.c. Its structure (Figure 7 a,b) is a complex aluminosilicate framework of three different types of secondary building units (Figure 7 c) linked into two interpenetrating pcu (primitive cubic) nets (Figure 7 d,e) connected by additional T nodes. The most reasonable explanation of zeolite complexity is their growth by self-assembly of prenucleation nanoclusters Angew. Chem. Int. Ed. 2014, 53, 654 – 661

Figure 7. The structure of paulingite viewed along the a axis (a) and the nodal representation of its tetrahedral framework (b). The framework can be considered as consisting of cages (c) that share edges to form a three-dimensional framework (d). Two frameworks interpenetrate and are linked by additional nodes (not shown) to form a complete paulingite topology (e).

already existing in the crystallization media.[33] Among the zeolite framework topologies known to date,[34] the paulingite PAU framework is the second in its topological complexity (4763.456 bits/u.c.), after the SFV framework reported for the synthetic zeolite SSZ-57 (19 557.629 bits/u.c.).[35] In general, oxides and oxysalts comprise about 6 % of 2000 most complex inorganic structures (Figure 3). Borates are characterized by the intrinsic structural complexity, owing to the ability of the B3+ ion to occur in triangular and tetrahedral coordination environments in the same structure. Figure 8 a shows the disposition of the [B7O12]3 borate layers in the structure of Cs3B7O12.[36] Each layer consists of three sublayers. The sublayers 1 and 2 are identical and rather simple, whereas the sublayer 3 that links sublayers 1 and 2 contains triborate moieties of three geometrical types (Figure 8 b), which leads to the occurrence of the very long unitcell parameter of 59.911 . The resulting structure is very complex and its total information content equals to 6062.598 bits/u.c. The structure of Ba12(SiO3)6(CO3)5Cl2[37] is an interesting example of the case when structural complexity is generated by the complex chemical composition. It can be described as being based upon rods of face-sharing (ClBa6) octahedra surrounded by (CO3)2 triangles, additional Ba2+ ions, and [SiO3] chains of corner-sharing SiO4 tetrahedra (Figure 9). The high complexity (IG,total = 3913.746 bits/u.c.) is created by the presence of both cation- and anion-centered[38] polyhedra

2014 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim

www.angewandte.org

659

. Angewandte Minireviews

S. V. Krivovichev

Figure 8. Arrangement of complex borate layers in the structure Cs3B7O12 (a; each layer can be subdivided into three sublayers: 1, 2, and 3) and projection of the layer 3 that shows that the groups indicated by red circles are translationally non-equivalent (b).

Figure 9. The crystal structure of Ba12(SiO3)6(CO3)5Cl2 (a) contains [ClBa3]5+ chains of face-sharing ClBa6 octahedra surrounded by (CO3)2 triangles (b), Ba2+ cations, and [SiO3] chains of corner-sharing SiO4 tetrahedra (c).

as the basic building units and their mutual arrangement in the resulting structure. In contrast to the oxo compounds, the number of very complex chalcogenides (e.g., sulfides and selenides) is much smaller. One of a few examples is the structure of ICF-26 (Figure 10 a), consisting of two interpenetrating mog-type frameworks formed by corner-sharing of [Li4In22S44]18 supertetrahedra (Figure 10 b). Similar to zeolites, the high complexity (IG,total = 5444.699 bits/u.c.) in this case is generated by the presence of nanoscale building blocks that self-assemble into a structure with relatively simple overall topology (Figure 10 c).

5. Summary and Perspectives Quantification of crystal-structure complexity using information theory allows basic mechanisms to be identified that are responsible for the appearance of complex structures in inorganic systems. The first and the most obvious one is a combination of chemically different components taken in complex proportions [e.g., in the intermetallic Al55.4Cu5.4Ta39.1 (ACT-71) or Ba12(SiO3)6(CO3)5Cl2]. This approach usually

660

www.angewandte.org

Figure 10. Structure of the In–Li sulfide ICF-26 composed from two interpenetrating frameworks (a) formed by corner-linkage of [Li4In22S44]18 supertetrahedra (b). Both frameworks have a rather simple moganite topology (c). Pink InS4 tetrahedra, blue LiS4 tetrahedra.

leads to the association, in the same structure, of different building blocks that can be considered as being extracted from the parent solids of higher structural simplicity. This feature of inorganic structures is known as modularity and has been widely applied to the description of complex materials.[39] Another complexity-generating mechanism depends upon the presence in the crystallization media (solution, melt, gas, etc.) of clusters of high nuclearity that self-assemble to form highly ordered three-dimensional crystalline arrays. This group of complex structures includes different kinds of polyoxometallates, cluster compounds, and fullerene-containing inorganic solids. It is very probable that the same mechanism is at work in the crystallization of porous frameworks containing various types of large building blocks (e.g., zeolites and microporous sulfide frameworks). Finally, complexity may be generated by local rather than global bonding requirements in compounds with simple chemical compositions. In this case, topologically simple frameworks acquire high structural complexity owing to the local atomic ordering and formation of superstructures and superlattices on cooling. Identification of structural complexity with information encoded in the atomic arrangement and its density allows relations between information and kinetics and thermodynamic parameters in crystalline materials to be quantitatively examined. For instance, quantitative verification can be made for the principle of “simplexity”,[40] which states that, in the course of fast processes, such as spontaneous crystallization at non-equilibrium conditions, structurally simpler metastable phases form more easily that their more complex but stable counterparts.[16d] Another interesting problem is the behavior of information along the path of phase transitions induced by changing pressure and temperature. Probably, the most fundamental question of interest is the relation between information and energy[41] in processes that involve transformations of crystalline phases. It should be stressed that the

2014 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim

Angew. Chem. Int. Ed. 2014, 53, 654 – 661

Angewandte

Chemie

Inorganic Crystal Structures

information content (or information entropies) of crystal structures considered herein are not identical to the thermodynamic entropies of the corresponding solids and to the information content employed in the statistical mechanics; the relations between these parameters are presently unclear. All these problems are far beyond the topic of this Minireview and require further exploration. I am indebted to Prof. V. A. Blatov for incorporation of information-based complexity measures into the TOPOS program package. This work was supported by the Russian Federal Grant-in-Aid Program “Cadres” (agreement no. 8313) and Russian Foundation for Basic Research (grant 13-0500928).

[16]

[17]

[18] [19] [20] [21] [22]

Received: May 21, 2013 Revised: July 6, 2013 Published online: December 13, 2013

[23] [24]

[1] J.-M. Lehn, Angew. Chem. 2013, 125, 2906 – 2921; Angew. Chem. Int. Ed. 2013, 52, 2836 – 2850. [2] a) J. Avery, Information Theory and Evolution, World Scientific, Singapore, 2003; b) Complexity in Chemistry, Biology, and Ecology (Eds.: D. Bonchev, D. H. Rouvray), Springer, New York, 2005; c) Information and The Nature of Reality, From Physics and Metaphysics (Eds.: P. Davies, N. Gregersen), Cambridge University Press, Cambridge, 2010; d) D. J. Graham, Chemical Thermodynamics and Information Theory with Applications, CRC, Taylor & Francis, Boca Raton, 2011. [3] E. Shannon, W. Weaver, The Mathematical Theory of Communications, University of Illinois Press, Urbana, 1949. [4] a) O. Goldreich, Computational Complexity: A Conceptual Perpective, Cambridge University Press, Cambridge, 2008; b) A. Sanjeev, B. Boaz, Computational Complexity: A Modern Approach, Cambridge University Press, Cambridge, 2009. [5] C. H. Bennet in Complexity, Entropy, and the Physics of Information, Santa Fe Institute Studies in the Sciences of Complexity (Ed.: W. H. Zurek), Vol. VIII, Addison-Wesley, 1990, pp. 137 – 148. [6] a) M. J. Buerger, V. Venkatakrishnan, Proc. Natl. Acad. Sci. USA 1974, 71, 4348 – 4351; b) S. E. Lister, I. R. Evans, J. A. K. Howard, A. Coelho, J. S. O. Evans, Chem. Commun. 2004, 2540 – 2541; c) S. E. Lister, I. R. Evans, J. S. O. Evans, Inorg. Chem. 2009, 48, 9271 – 9281; d) L. Bindi, F. Nestola, A. Guastoni, L. Secco, Mineral. Mag. 2010, 74, 999 – 1012; e) C. Hoch, A. Simon, Angew. Chem. 2012, 124, 3316 – 3319; Angew. Chem. Int. Ed. 2012, 51, 3262 – 3265. [7] J. K. Burdett, C. Marians, J. F. Mitchell, Inorg. Chem. 1994, 33, 1848 – 1856. [8] L. Pauling, J. Am. Chem. Soc. 1929, 51, 1010 – 1026. [9] F. C. Hawthorne in Landmark Papers: Structure Topology (Ed.: F. C. Hawthorne), The Mineralogical Society of Great Britain and Ireland, Twickenham, 2006, p. L12. [10] W. H. Baur, E. T. Tillmanns, W. Hofmeister, Acta Crystallogr. Sect. B 1983, 39, 669 – 674. [11] A. L. Mackay, J. Klinowski, Comp. Math. Appl. Part B 1986, 12, 803 – 824. [12] A. L. Mackay, Crystallogr. Rep. 2001, 46, 524 – 526. [13] E. Estevez-Rams, R. Gonzlez-Frez, Z. Kristallogr. 2009, 224, 179 – 184. [14] W. Steurer, Acta Crystallogr. Sect. A 2011, A67, C184. [15] a) N. Rashevsky, Bull. Math. Biophys. 1955, 17, 229 – 235; b) E. Trucco, Bull. Math. Biophys. 1956, 18, 129 – 135; c) D. Bonchev,

Angew. Chem. Int. Ed. 2014, 53, 654 – 661

[25]

[26] [27] [28]

[29]

[30] [31] [32] [33]

[34] [35] [36] [37] [38] [39]

[40] [41]

SAR QSAR Environ. Res. 2003, 14, 199 – 214; d) M. Dehmer, A. Mowshowitz, Inform. Sci. 2011, 181, 57 – 78. a) S. V. Krivovichev, Acta Crystallogr. Sect. A 2012, 68, 393 – 398; b) S. V. Krivovichev, Struct. Chem. 2012, 23, 1045 – 1052; c) S. V. Krivovichev, Microporous Mesoporous Mater. 2013, 171, 223 – 229; d) S. V. Krivovichev, Miner. Mag. 2013, 77, 275 – 326. T. J. R. Weakley, E. R. Ylvisaker, R. J. Yager, J. E. Stephens, R. D. Wiegel, M. Mengis, P. Wu, P. Photinos, S. C. Abrahams, Acta Crystallogr. Sect. B 2004, 60, 705 – 715. S. V. Krivovichev, E. V. Kir’yanova, S. K. Filatov, P. C. Burns, Acta Crystallogr. Sect. C 2000, 56, 629 – 630. G.-C. Guo, W.-D. Cheng, J.-T. Chen, H.-H. Zhuang, J.-S. Huang, Q.-E. Zhang, Acta Crystallogr. Sect. C 1995, 51, 2469 – 2471. A. K. Pant, Acta Crystallogr. Sect. B 1968, 24, 1077 – 1083. P. J. Mohr, B. N. Taylor, D. B. Newell, Rev. Mod. Phys. 2008, 80, 633 – 730. Inorganic Crystal Structure Database. FIZ Karlsruhe GmbH 2012. V. A. Blatov, A. P. Shevchenko, V. N. Serezhkin, J. Appl. Crystallogr. 2000, 33, 1193. T. Weber, J. Dshemuchadse, M. Kobas, M. Conrad, B. Harbrecht, W. Steurer, Acta Crystallogr. Sect. B 2009, 65, 318 – 325. T. Mitra, P. Mir, A.-R. Tomsa, A. Merca, H. Bçgge, J. B. valos, J. M. Poblet, C. Bo, A. M ller, Chem. Eur. J. 2009, 15, 1844 – 1852. A. M ller, P. Gouzerh, Chem. Soc. Rev. 2012, 41, 7431 – 7463. a) P. C. Burns, Miner. Mag. 2011, 75, 1 – 25; b) J. Qiu, P. C. Burns, Chem. Rev. 2013, 113, 1097 – 1120. a) T. Z. Forbes, J. G. McAlpin, R. Murphy, P. C. Burns, Angew. Chem. 2008, 120, 2866 – 2869; Angew. Chem. Int. Ed. 2008, 47, 2824 – 2827; b) G. E. Sigmon, D. K. Unruh, J. Ling, B. Weaver, M. Ward, L. Pressprich, A. Simonetti, P. C. Burns, Angew. Chem. 2009, 121, 2775 – 2778; Angew. Chem. Int. Ed. 2009, 48, 2737 – 2740; c) J. Ling, C. M. Wallace, J. E. S. Szymanowski, P. C. Burns, Angew. Chem. 2010, 122, 7429 – 7431; Angew. Chem. Int. Ed. 2010, 49, 7271 – 7273. C. A. Ohlin, E. M. Villa, J. C. Fettinger, W. H. Casey, Angew. Chem. 2008, 120, 5716 – 5718; Angew. Chem. Int. Ed. 2008, 47, 5634 – 5636. B. S. Guiton, H. Wu, P. K. Davies, Chem. Mater. 2008, 20, 2860 – 2862. G. Costentin, A. Leclaire, M. M. Borel, A. Grandin, B. Raveau, Z. Kristallogr. 1992, 201, 53 – 58. E. K. Gordon, S. Samson, W. B. Kamb, Science 1966, 154, 1004 – 1007. A. Depla, E. Verheyen, A. Veyfeyken, M. Van Houteghem, K. Houthoofd, V. Van Speybroeck, M. Waroquier, C. E. A. Kirschhock, J. A. Martens, J. Phys. Chem. C 2011, 115, 11077 – 11088. C. Baerlocher, L. B. McCusker, D. H. Olson, Atlas of Zeolite Framework Types, 6th ed., Elsevier, Amsterdam, 2007. C. Baerlocher, T. Weber, L. B. McCusker, L. Palatinus, S. I. Zones, Science 2011, 333, 1134 – 1137. G. Nowogrocki, N. Penin, M. Touboul, Solid State Sci. 2003, 5, 795 – 803. A. M. Il’yinets, Yu. A. Malinovskii, Dokl. Akad. Nauk SSSR 1985, 282, 890 – 894. S. V. Krivovichev, O. Mentre, O. I. Siidra, M. Colmont, S. K. Filatov, Chem. Rev. 2013, 113, 6459 – 6535. a) G. Ferraris, E. Mackovicky, S. Merlino, Crystallography of Modular Materials, Oxford University Press, Oxford, 2004; b) M. G. Kanatzidis, Acc. Chem. Res. 2005, 38, 359 – 368. J. R. Goldsmith, J. Geol. 1953, 61, 439 – 451. a) R. Landauer, Phys. Lett. A 1996, 217, 188 – 193; b) A. Brut, A. Arakelyan, A. Petrosyan, S. Ciliberto, R. Dillenschneider, E. Lutz, Nature 2012, 483, 187 – 190.

2014 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim

www.angewandte.org

661

S. V. Krivovichev

DOI: 10.1002/anie.201304374

Inorganic Crystal Structures

Which Inorganic Structures are the Most Complex? Sergey V. Krivovichev* crystallography · information theory · inorganic structures · structural complexity · structural elucidation

The discovery of the diffraction of X-rays on crystals opened up a new era in our understanding of nature, leading to a multitude of striking discoveries about the structures and functions of matter on the atomic and molecular scales. Over the last hundred years, about 150 000 of inorganic crystal structures have been elucidated and visualized. The advent of new technologies, such as area detectors and synchrotron radiation, led to the solution of structures of unprecedented complexity. However, the very notion of structural complexity of crystals still lacks an unambiguous quantitative definition. In this Minireview we use information theory to characterize complexity of inorganic structures in terms of their information content.

1. Introduction The evolution of matter towards states of higher complexity in the course of the evolution of the Universe is one of the most interesting topics in modern science and in modern chemistry in particular.[1] A number of different approaches exist that allow the complexity of chemical, biological, technological, and even social systems to be quantitatively evaluated.[2] Most of these approaches are based upon the extensive use of concepts and techniques borrowed from the information theory developed in the second half of the 20th century as a theory of communication and transmission of information.[3] Nowadays complexity theory is a well-developed field of computer science with interdisciplinary applications in many areas of theoretical and applied sciences.[4] It is interesting, however, that complexity theorists have always regarded crystals as “intuitively simple objects”,[5] in contrast to much more complex and dynamic biological systems. On the other hand, it was largely appreciated that crystal structures may possess different degrees of complexity, which has been reflected in the titles of scientific papers with the use of expressions such as “complicated structure”, “the most complex structure”, “complexity”, “complex superstructures”, “a masterpiece of structural complexity”.[6] However, until recently, the complexity of crystal structures was

[*] Prof. Dr. S. V. Krivovichev Department of Crystallography, St. Petersburg State University University Emb. 7/9, 199034 St. Petersburg (Russia) E-mail: [email protected]

654

destined to be “largely a qualitative, frequently intuitive, notion”,[7] which escaped a quantitative definition. Perhaps, the first attempt to evaluate structural complexity of crystals should be assigned to the Linus Paulings fifth (“parsimony”) rule “determining the structure of complex ionic crystals”:[8] “the number of different types of constituents in a crystal tends to be small.” Hawthorne[9] noted that “this rule has not seen much use, apart from in teaching, but it certainly seems to hold reasonably well, and its underlying cause is certainly of interest.” The certain advantage of crystals is that their almost infinite network of atoms and bonds can be described by a rather small volume of space called the elementary unit cell. Of even smaller volume is the asymmetric unit, which only contains symmetrically inequivalent atoms. To provide a quantitative definition of crystal-structure complexity, Baur et al.[10] suggested to use topological and crystallographic parsimony indices, It and Ic, defined by Equations (1) and (2), I t ¼ ðteÞ=t

ð1Þ

I c ¼ ðceÞ=c

ð2Þ

where e is the number of different chemical elements, and t and c are the numbers of topologically and crystallographically distinct atom sites in the asymmetric unit, respectively. Baur et al.[10] pointed out that the topological parsimony index is of primary importance and suggested subdividing structures into lavish (It > 0.66), intermediate (0.66 > It > 0.33), and parsimonius (It < 0.33). Both indices are not sensitive either to chemical complexity or symmetry and reflect only relations between the number of chemical elements and the number of topologically or crystallographically distinct atom sites.

2014 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim

Angew. Chem. Int. Ed. 2014, 53, 654 – 661

Angewandte

Chemie

Inorganic Crystal Structures

An alternative approach to structural complexity was suggested by Lister et al.,[6b,c] who used the number of atoms in the asymmetric unit as a measure of complexity for a commensurate structure. This method has many advantages but, unfortunately, does not provide an appropriate quantification of the complexity of high-symmetry structures, such as, paulingite, a complex natural zeolite, which was identified by Mackay and Klinowski[11] as one of the most complex inorganic structure. Mackay[12] and later Estevez-Rams and Gonzlez-Frez[13] proposed to estimate the complexity of crystal structures on the basis of the complexity of algorithms that can be used to generate them from an unordered array of atoms. This concept is of great interest, but, in its present state, requires a high level of abstraction and imagination and cannot be applied to crystal structures in an easy and unambiguous way. In this Minireview, a different method is employed to evaluate the complexity of structures, which is based upon the relatively simple application of Shannon information theory and allows both size- and symmetry-dependent properties of complex structures to be quantitatively evaluated, thus combining their symbolic and combinatorial complexities[14] in the same measure.

2. Basic Concepts In the framework of classical information theory, information content H of a message M consisting of v symbols that belong to the k equivalence classes is calculated according to the following Shannon formula [Eq. (3)] H¼

k X

pi log2 pi ½bits=symbol

ð3Þ

i¼1

subdivided into equivalence classes according to their crystallographic orbits, that is, two atoms belong to the same class if they are symmetrically equivalent. This led to the following formula to calculate the structural information content, IG, of a crystal structure [Eq. (5)] IG ¼

k X

where k is the number of crystallographic orbits and pi is the probability of occurrence of the atom of the ith crystallographic orbit [Eq. (6)] pi ¼ mi =v

ð6Þ

where mi is the multiplicity of the crystallographic orbit relative to the reduced unit cell, and v is the number of atoms in the reduced unit-cell. For instance, the structure of lopezite, K2Cr2O7,[17] is triclinic, space group P1¯. All the atoms in the structure occupy 2i Wyckoff sites: there are four K, four Cr, and fourteen O sites, which corresponds to the total number of 22 equivalence classes. The total number of atoms in the reduced unit cell (which in this case coincides with the crystallographic unit cell) is 44. Atoms from each equivalence class has the same probability of occurrence, which is equal to 2/44 = 0.0455. The structural information content for lopezite is given by Equation (7). I G ¼ 22 ð2=44Þ log2 2=44 ¼ 4:459 bits=atom

pi ¼ mi =v

ð4Þ

where mi is the number of symbols in M that belong to the ith equivalence class. Following theoretical works on the topological complexity of graphs and networks,[2b, 15] Krivovichev[16] proposed to consider the reduced elementary unit cell of a crystal structure as a message consisting of v atoms. The atoms are

Sergey Krivovichev received his Ph.D. (1997) and D.Sc. (2002) degrees from St. Petersburg State University and carried our post-doctoral research in the U.S., Germany, Switzerland, and Austria. Since 2005, he is a Full Professor and Chairman of Department of Crystallography, St. Petersburg State University. His research interests include inorganic structural chemistry, mineralogy, crystallography, nuclear materials, and applications of complexity theory to natural and artificial objects.

Angew. Chem. Int. Ed. 2014, 53, 654 – 661

ð7Þ

The total information content of a crystal structure is determined by the Equation (8). I G,total ¼ v I G ðbits=unit-cellÞ

where pi is the probability of occurrence of the ith symbol [Eq. (4)]:

ð5Þ

pi log2 pi ½bits=atom

i¼1

ð8Þ

For lopezite, IG,total = 44 4.459 = 196.196 bits per unit-cell (bits/u.c.). The maximal structural information content, IG,max, for a crystal structure with v atoms occurs, where all atoms are non-equivalent according to the corresponding space group. It can be calculated as Equation (9). I G,max ¼ log2 v ðbits=atomÞ

ð9Þ

For IG to be independent of v, we may define the normalized structural information content, IG,norm, as Equation (10). I G,norm ¼ I G =I G,max ¼ ½

k X

pi log2 pi =log2 v

ð10Þ

i¼1

For the structure of lopezite, IG,max = log2 44 = 5.459 bits/atom and IG,norm = 4.459/5.459 = 0.817. Note that IG,norm is a dimensionless quantity in the range from 0 to 1. The information-based complexity measures allow us to introduce the concept of information density, which can be defined as a number of bits of information per cubic ngstrçm [Eq (11)].

2014 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim

www.angewandte.org

655

. Angewandte Minireviews 1inf ¼ I G,total =V ðbits 3 Þ

S. V. Krivovichev

ð11Þ

BaTiO3 is more complex than rutile, TiO2 (rutile), whereas rutile is more complex than NaCl (halite). Both parsimony For lopezite, 1inf = 0.270 bits 3. For another modification of indices, It and Ic,[10] cannot discriminate between the complex[18] 3 K2Cr2O7, 1inf = 0.156 bits , which indicates its lower ities of the three structures, whereas the number of atoms complexity compared to lopezite. It is important that within the asymmetric unit (c)[6b,c] cannot distinguish between information density should be calculated using the volume the complexities of tetragonal rutile and cubic halite. On the of the reduced unit cell. other hand, ranking of the structures according to the IG,total For two structures with similar unit cells but different values is in agreement with the intuitive feelings (in bits per symmetry, information density will be higher for the structure unit cell): 6.855 (BaTiO3) > 5.510 (rutile) > 2.000 (halite). In with lower symmetry (and higher complexity). For instance, general, it may be concluded that the parsimony indices[10] do cation ordering within the same unit cell would lead to the not possess enough discriminative power, whereas the c formation of a superstructure with higher information density parameter underestimates complexities of highly symmetrical than that of the original structure. This situation shows that structures and structures with non-general orbits. unit-cell volume alone cannot be considered as a measure of Since total information content of the crystal structure, structural complexity, since it reflects only the symbolic IG,total, is defined per unit cell, it is possible to calculate a total complexity of the system and is not sensitive to its combinainformation amount of a particular crystal. For instance, torial complexity. a 1 mole crystal of a-quartz, space group P3221, Z = 3, Information density can also be used as a measure of contains approximately 2.00738 1023 unit cells calculated as complexity for the crystal structures of solids with similar the Avogadro number, 6.02214 1023,[21] divided by Z = 3. The composition. The fact that complexity is a function of both total information content of the crystal structure of a-quartz is information content and unit-cell volume makes it dependent IG,total = 8.265 bits/u.c. Therefore, the total information conupon the size of atoms and ions that make up the respective tent of the 1 mole quartz crystal is equal to approximately crystal, as well as upon temperature and pressure. Suanite, 16.59100 1023 bits. It should be emphasized that, clearly, [19] [20] Mg2B2O5, and natrosilite, Na2Si2O5, have the same total structural information of a crystal consisting of billions of unit cells is redundant or algorithmically compressible.[12] Neverstructural information content (114.117 bits/u.c.), but their information densities are drastically different (0.333 and theless, the full amount of this (redundant) information can 0.242 bits 3, respectively), which is a consequence of the be calculated from the amount of the respective crystalline substance expressed either in molar, mass, or volumnar different ionic radii of the Mg2+ and Na+ ions, on the one quantities. This means that, similar to mass, entropy, volume, hand, and of the B3+ and Si4+ ions, on the other. However, for example, information is an “extensive” property as while information density cannot be used to compare opposed to the “intensive” properties such as temperature structures with different chemical compositions, it is a useful and pressure. parameter for the investigation of behavior of structural To explain this point further, consider the following information in the course of phase transitions induced by sequences: a) 010101010101010101, b) 101001101001101001, temperature and pressure, that is, when chemical composition and c) 010001111000101101. To store these sequences, any is a constant parameter. computer would need exactly 18 bits for each, which means Table 1 presents comparison of the values of the complexthat the amount of information expressed in bits is identical ity parameters defined according to Baur et al.,[10] Lister for the three sequences. However, the sequence (c) cannot be et al.,[6b,c] and this work, applied to different simple and compressed, whereas the sequences (a) and (b) are algorithcomplex inorganic structures. These data indicate certain mically compressible: the sequence (a) can be represented as advantages in the use of information-based complexity “repeat 01 nine times”, whereas (b) as “repeat 101001 three parameters (and, in particular, the IG,total parameter) as times”. By analogy, crystals can be constructed by repeating compared to the purely crystallographic parameters (v, c, It, its unit cell in a three-dimensional space; however, its full and Ic). For instance, according to the intuitive feelings, information content will be a function of the number of these repeats, just as the full information content Table 1: Comparison of the values of different complexity parameters for the same inorganic crystal of the sequence (b) is the function structures of the number of repeats of the Structure ICSD v c It[c] Ic[d] IG IG,total IG,norm sequence “101001”. It can be ar[a] [b] code [atoms] [atoms] [bits] [bits/u.c.] gued that, in the framework of this NaCl 53815 2 2 0 0 1.000 2.000 1.000 approach, a piece of glass would 53997 6 2 0 0 0.918 5.510 0.355 TiO2 rutile contain more information than the BaTiO3 cubic 56093 5 3 0 0 1.371 6.855 0.590 crystal with the corresponding com36261 24 7 0 0.71 2.752 66.039 0.600 SiO2 coesite Ba2Ti9O20 35711 124 62 0.90 0.95 5.954 738.320 0.856 position, since, because of the abBa6Ti17O40 49576 126 34 0.89 0.91 5.057 637.137 0.725 sence of the long-range order, the SiP2O7 cubic 66861 1080 50 0 0.94 5.570 6015.280 0.553 structure of the glass is unique in Cu2Li2P6O18 2149 56 28 0.73 0.86 4.807 269.212 0.828 each point of the piece. However, [a] Number of atoms per reduced unit cell. [b] Number of atoms per asymmetric unit.[6b,c] [c] Topological this information is meaningless, since local distortion of the strucparsimony index.[10] [d] Crystallographic parsimony index.[10]

656

www.angewandte.org

2014 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim

Angew. Chem. Int. Ed. 2014, 53, 654 – 661

Angewandte

Chemie

Inorganic Crystal Structures

ture of the glass would not alter its properties. The IG value proposed above measures structural information per atom, whereas the IG,total value defines information amount per smallest unit, which forms the whole structure by its repeating in three dimensions. As can be seen from Table 1, the most adequate parameter to evaluate complexity of a crystal structure is IG,total.

3. Complexity of Inorganic Structures: Statistics To analyze the complexity of inorganic structures on a large-scale basis, complexity parameters have been calculated for all the crystal-structure entries stored in the Inorganic Crystal Structure Database (ICSD)[22] using the TOPOS program package.[23] Figure 1 shows distribution of

Figure 2. Diagrams showing relations between complexity parameters for the ICSD reports: number of atoms per unit cell (v), structural information content per atom (IG) and per unit cell (IG,total): point diagram (a); each point corresponds to a single ICSD report (two reports with IG,total > 35 000 bits are omitted for clarity) and a contour map (b) colors show the range of the IG,total values).

Figure 1. Histogram showing distribution of inorganic crystal-structure reports stored in the Inorganic Crystal Structure Database (ICSD) according to the values of the information-based IG and IG,total parameters.

the ICSD reports according to the information contents per atom (IG) and per unit-cell (IG,total). According to the IG,total values, all structures can be subdivided into very simple, simple, intermediate, complex, and very complex (Table 2). It can be seen from Figure 1 that most ICSD entries are for very simple and simple structures that together constitute about 75 % of the ICSD data. This reflects the fact that structurally and chemically simple inorganic compounds have been most studied over the last hundred years, though the general current trend is towards the elucidation of structures with increasing complexity (see below).

Table 2: Classification of inorganic crystal structures according to their complexity (information content per unit cell). Category

IG,total [bits/u.c.]

Number of ICSD entries

very simple simple intermediate complex very complex

< 20 20–100 100–500 500–1000 > 1000

ca. 55 000 ca. 50 000 ca. 33 000 ca. 5000 ca. 3000

Angew. Chem. Int. Ed. 2014, 53, 654 – 661

Figure 2 shows relations between the information contents per atom (IG) and per unit-cell (IG,total), and the number of atoms in the unit cell (v) (note that all the quantities are referred to the reduced unit cells). It can be seen that there is a general positive correlation between v and IG,total. However, structures with the same number of atoms per unit cell may differ in their IG,total values by several hundreds of bits, which shows that, in agreement with the previous conclusion, the purely crystallographic v parameter cannot be used as a single complexity measure, since it accounts for the size of the structure only, and not for its symmetry. The symmetrysensitive parameter is IG, and the IG,total parameter provides combination of both size- and symmetry-sensitive complexity measures.

4. Most Complex Inorganic Structures Analysis of the 2000 most-complex structures stored in the ICSD according to their belonging to specific classes of inorganic compounds is shown in Figure 3. About 90 % of all these compounds are structures based upon nanoscale-sized clusters with 82 % represented by Mo-, W-, and V-based polyoxometallates. Among other classes are: oxides and oxysalts (e.g., silicates, sulfates, borates), zeolites and microporous framework materials, intermetallic compounds, borides and silicides, superstructures of simpler structure types, sulfides and selenides, and halogenides. The most complex inorganic structure reported to date is that of the intermetallic compound Al55.4Cu5.4Ta39.1 (ACT-

2014 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim

www.angewandte.org

657

. Angewandte Minireviews

S. V. Krivovichev

Figure 3. Classification of the 2000 most-complex inorganic structures according to their chemical identity: 1) Mo-, W-, V-based polyoxometallates; 2) oxides and oxysalts; 3) structures containing (nano)clusters; 4) zeolites and microporous framework compounds; 5) intermetallic compounds (including borides and silicides); 6) fullerene-based structures; 7) uranyl peroxide nanospheres; 8) superstructures of simple structure types; 9) Nb-, Ti-based polyoxometallates; 10) sulfides and selenides; 11) halogenides.

71).[24] Its total structural information content is equal to 48 538.637 bits/u.c. The reduced unit cell contains v = 5814 atom sites and the structural information content per atom (IG) is 8.349 bits. The exceptional complexity of this structure is the result of the combination of different structural modules, which was described by Steurer and coworkers[24] as follows: The Al12Ta28 fullerene cluster shells (orange polyhedra in Figure 4 a consisting of 40 faces and 76 vertices) are linked by the Ta15 bifrusta (red polyhedra consisting of 12 faces and 15 vertices) into a porous framework with large cavities occupied by supertetrahedral clusters of two types. The first type (Figure 4 b,c) consists of 146 Tacentered Al12 Friauf polyhedra, Ta8 hexagonal bipyramids, and Al12Ta28 fullerene shells. The second type is formed by ten Al102Ta57 fullerenes (Figure 4 e). The supertetrahedral clusters

Figure 4. Structural building principle of Al55.4Cu5.4Ta39.1 (ACT-71). Reproduced with permission from Ref. [24].

658

www.angewandte.org

form two interpenetrating diamond-type networks (Figure 4 d) and, together with the fullerene–bifrustum framework (Figure 4 a), form the unit cell of extraordinary complexity (Figure 4 f). The second most complex structure is that of (C(NH2)3)136[{(C(NH2)3)20(H2O)100}{(Mo)Mo5O21(H2O)6}12{Mo2O4(H2PO2)}20{Mo2O4(SO4)}10][{(C(NH2)3)20(H2O)80} {(Mo)Mo5O21(H2O)6}12{Mo2O4(H2PO2)}12{Mo2O4(SO4)}18](H2O)400,[25] which contains spherical polyoxomolybdate cluster of the type {(Mo)Mo5}12(spacer)30 (one of the “Keplerates”)[26] (Figure 5 a,b). The nanocavity inside the cluster is occupied by the (H2O)100 nanodrop of water with H2O

Figure 5. Polyoxometalates nanoscale clusters from selected very complex inorganic structures (skeletal representation is given for each cluster showing the topology of the metal-O-metal links): a,b) “Keplerate” cluster from the structure of {[(NH2)3C]52}{(Mo)Mo5O21(H2O)6}12 {Mo2O4(SO4)}10{Mo2O4(H2PO2)}20 (pink and red polyhedra are Mo and P coordination polyhedra, respectively); c,d) uranyl peroxide nanosphere with the C50 fullerene topology (yellow polyhedra are uranyl hexagonal bipyramids); e,f) 18-nuclear Ti-Nb-polyoxometalate cluster from the structure of [N(CH3)4]20[Ti12Nb6O44]2(H2O)73 (Ti and Nb polyhedra are shown as blue and green, respectively).

molecules arranged in three concentric shells. The enormous complexity (IG,total = 45341.050 bits/u.c., v = 5128 atoms/u.c.) is not only due to the size of the clusters, but also due to the fact that there are two crystallographically independent clusters in the structure with 3¯m and 2/m site symmetries. Very complex structures with giant clusters are dominated by Mo-, W-, and V-polyoxometallates. However, oxo-nanoclusters of other metals can also assemble to form structures of high complexity. A prominent example is the uranyl peroxide nanospheres formed by linkage of uranyl ions, UO22+, through peroxide groups (Figure 5 c,d).[27] The maximal number of uranyl ions in such clusters prepared to date is 120, and some of the clusters adopt fullerene topologies.[28] It is noteworthy that uranyl peroxide nanospheres are porous and their cavities may accommodate various cations and H2O molecules. Figure 5 e shows the [Ti12Nb6O44]10 cluster from the structure of [N(CH3)4]20[Ti12Nb6O44]2(H2O)73.[29] Despite the obvious high symmetry of the cluster (m3¯m) that can be appreciated from its skeletal representation (Figure 5 f), the symmetry of the crystal structure is monoclinic (space group P21/c).

2014 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim

Angew. Chem. Int. Ed. 2014, 53, 654 – 661

Angewandte

Chemie

Inorganic Crystal Structures

Figure 6. The nanoscale-domain superstructure of Nd7/12Li1/4TiO3 consisting of square-shaped Li-rich regions (white) separated by zigzagging boundary regions of a Nd-rich structure (orange).

Another complexity-generating mechanism in inorganic materials is formation of superstructures either by atomic ordering or displacive phase transitions. Figure 6 shows an ordered nano-checkerboard superlattice observed in the structure of Nd7/12Li1/4TiO3 by transmission electron microscopy and modeled by Rietveld refinement.[30] The structure in general belongs to the perovskite structure type (ABO3) with Ti in the B site and Li and Nd in the A site. The Li–Nd ordering results in formation of square-shaped nanoscale domains of a Li-rich phase separated by a zig-zagging boundary region consisting of a Nd-rich phase.[30] The resulting supercell has the dimensions 14ap 28ap 2ap, where ap is the unit-cell parameter of a simple perovskite. The total information content of the structure equals to 16 634.804 bits/ u.c. with v = 1973 atoms/u.c. An example of a very complex structure with complexity generated by displacive phase transitions on cooling is that of [Mo2P4O15] which can be written as [(MoO)2P4O13].[6b,c] The structure consists of corner-sharing MoO6 octahedra interlinked by linear P4O13 tetramers of tetrahedra. Its topological complexity (i.e., complexity of an archetype framework) is rather small (IG,total = 144.477 bits/u.c.),[31] whereas real structures are very complex (7748.048 bits/u.c. for monoclinic 120 K a-phase and 4022.549 bits/u.c. for triclinic 573 K bphase).[6b,c] The high complexity of the real structures compared to the much simpler archetype is due to the local bonding requirements that led to the formation of extended superstructures. This example is remarkable in that the symmetry of a high-temperature b-phase (space group P1¯) is lower than the symmetry of a low-temperature a-phase (space group Pn). However, the information amount of the high-temperature phase is smaller than that of the lowtemperature phase, which shows that, at least in this case, the information amount decreases with the increasing temperature, despite the decreasing symmetry. The high topological and structural complexity of zeolites and microporous oxide-based frameworks has long been recognized. One of the most complex zeolites[16c] and the most complex mineral known to date[16d] is paulingite, K6Ca16(Al38Si130O336)(H2O)113,[32] with IG,total = 6766.998 bits/ u.c. Its structure (Figure 7 a,b) is a complex aluminosilicate framework of three different types of secondary building units (Figure 7 c) linked into two interpenetrating pcu (primitive cubic) nets (Figure 7 d,e) connected by additional T nodes. The most reasonable explanation of zeolite complexity is their growth by self-assembly of prenucleation nanoclusters Angew. Chem. Int. Ed. 2014, 53, 654 – 661

Figure 7. The structure of paulingite viewed along the a axis (a) and the nodal representation of its tetrahedral framework (b). The framework can be considered as consisting of cages (c) that share edges to form a three-dimensional framework (d). Two frameworks interpenetrate and are linked by additional nodes (not shown) to form a complete paulingite topology (e).

already existing in the crystallization media.[33] Among the zeolite framework topologies known to date,[34] the paulingite PAU framework is the second in its topological complexity (4763.456 bits/u.c.), after the SFV framework reported for the synthetic zeolite SSZ-57 (19 557.629 bits/u.c.).[35] In general, oxides and oxysalts comprise about 6 % of 2000 most complex inorganic structures (Figure 3). Borates are characterized by the intrinsic structural complexity, owing to the ability of the B3+ ion to occur in triangular and tetrahedral coordination environments in the same structure. Figure 8 a shows the disposition of the [B7O12]3 borate layers in the structure of Cs3B7O12.[36] Each layer consists of three sublayers. The sublayers 1 and 2 are identical and rather simple, whereas the sublayer 3 that links sublayers 1 and 2 contains triborate moieties of three geometrical types (Figure 8 b), which leads to the occurrence of the very long unitcell parameter of 59.911 . The resulting structure is very complex and its total information content equals to 6062.598 bits/u.c. The structure of Ba12(SiO3)6(CO3)5Cl2[37] is an interesting example of the case when structural complexity is generated by the complex chemical composition. It can be described as being based upon rods of face-sharing (ClBa6) octahedra surrounded by (CO3)2 triangles, additional Ba2+ ions, and [SiO3] chains of corner-sharing SiO4 tetrahedra (Figure 9). The high complexity (IG,total = 3913.746 bits/u.c.) is created by the presence of both cation- and anion-centered[38] polyhedra

2014 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim

www.angewandte.org

659

. Angewandte Minireviews

S. V. Krivovichev

Figure 8. Arrangement of complex borate layers in the structure Cs3B7O12 (a; each layer can be subdivided into three sublayers: 1, 2, and 3) and projection of the layer 3 that shows that the groups indicated by red circles are translationally non-equivalent (b).

Figure 9. The crystal structure of Ba12(SiO3)6(CO3)5Cl2 (a) contains [ClBa3]5+ chains of face-sharing ClBa6 octahedra surrounded by (CO3)2 triangles (b), Ba2+ cations, and [SiO3] chains of corner-sharing SiO4 tetrahedra (c).

as the basic building units and their mutual arrangement in the resulting structure. In contrast to the oxo compounds, the number of very complex chalcogenides (e.g., sulfides and selenides) is much smaller. One of a few examples is the structure of ICF-26 (Figure 10 a), consisting of two interpenetrating mog-type frameworks formed by corner-sharing of [Li4In22S44]18 supertetrahedra (Figure 10 b). Similar to zeolites, the high complexity (IG,total = 5444.699 bits/u.c.) in this case is generated by the presence of nanoscale building blocks that self-assemble into a structure with relatively simple overall topology (Figure 10 c).

5. Summary and Perspectives Quantification of crystal-structure complexity using information theory allows basic mechanisms to be identified that are responsible for the appearance of complex structures in inorganic systems. The first and the most obvious one is a combination of chemically different components taken in complex proportions [e.g., in the intermetallic Al55.4Cu5.4Ta39.1 (ACT-71) or Ba12(SiO3)6(CO3)5Cl2]. This approach usually

660

www.angewandte.org

Figure 10. Structure of the In–Li sulfide ICF-26 composed from two interpenetrating frameworks (a) formed by corner-linkage of [Li4In22S44]18 supertetrahedra (b). Both frameworks have a rather simple moganite topology (c). Pink InS4 tetrahedra, blue LiS4 tetrahedra.

leads to the association, in the same structure, of different building blocks that can be considered as being extracted from the parent solids of higher structural simplicity. This feature of inorganic structures is known as modularity and has been widely applied to the description of complex materials.[39] Another complexity-generating mechanism depends upon the presence in the crystallization media (solution, melt, gas, etc.) of clusters of high nuclearity that self-assemble to form highly ordered three-dimensional crystalline arrays. This group of complex structures includes different kinds of polyoxometallates, cluster compounds, and fullerene-containing inorganic solids. It is very probable that the same mechanism is at work in the crystallization of porous frameworks containing various types of large building blocks (e.g., zeolites and microporous sulfide frameworks). Finally, complexity may be generated by local rather than global bonding requirements in compounds with simple chemical compositions. In this case, topologically simple frameworks acquire high structural complexity owing to the local atomic ordering and formation of superstructures and superlattices on cooling. Identification of structural complexity with information encoded in the atomic arrangement and its density allows relations between information and kinetics and thermodynamic parameters in crystalline materials to be quantitatively examined. For instance, quantitative verification can be made for the principle of “simplexity”,[40] which states that, in the course of fast processes, such as spontaneous crystallization at non-equilibrium conditions, structurally simpler metastable phases form more easily that their more complex but stable counterparts.[16d] Another interesting problem is the behavior of information along the path of phase transitions induced by changing pressure and temperature. Probably, the most fundamental question of interest is the relation between information and energy[41] in processes that involve transformations of crystalline phases. It should be stressed that the

2014 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim

Angew. Chem. Int. Ed. 2014, 53, 654 – 661

Angewandte

Chemie

Inorganic Crystal Structures

information content (or information entropies) of crystal structures considered herein are not identical to the thermodynamic entropies of the corresponding solids and to the information content employed in the statistical mechanics; the relations between these parameters are presently unclear. All these problems are far beyond the topic of this Minireview and require further exploration. I am indebted to Prof. V. A. Blatov for incorporation of information-based complexity measures into the TOPOS program package. This work was supported by the Russian Federal Grant-in-Aid Program “Cadres” (agreement no. 8313) and Russian Foundation for Basic Research (grant 13-0500928).

[16]

[17]

[18] [19] [20] [21] [22]

Received: May 21, 2013 Revised: July 6, 2013 Published online: December 13, 2013

[23] [24]

[1] J.-M. Lehn, Angew. Chem. 2013, 125, 2906 – 2921; Angew. Chem. Int. Ed. 2013, 52, 2836 – 2850. [2] a) J. Avery, Information Theory and Evolution, World Scientific, Singapore, 2003; b) Complexity in Chemistry, Biology, and Ecology (Eds.: D. Bonchev, D. H. Rouvray), Springer, New York, 2005; c) Information and The Nature of Reality, From Physics and Metaphysics (Eds.: P. Davies, N. Gregersen), Cambridge University Press, Cambridge, 2010; d) D. J. Graham, Chemical Thermodynamics and Information Theory with Applications, CRC, Taylor & Francis, Boca Raton, 2011. [3] E. Shannon, W. Weaver, The Mathematical Theory of Communications, University of Illinois Press, Urbana, 1949. [4] a) O. Goldreich, Computational Complexity: A Conceptual Perpective, Cambridge University Press, Cambridge, 2008; b) A. Sanjeev, B. Boaz, Computational Complexity: A Modern Approach, Cambridge University Press, Cambridge, 2009. [5] C. H. Bennet in Complexity, Entropy, and the Physics of Information, Santa Fe Institute Studies in the Sciences of Complexity (Ed.: W. H. Zurek), Vol. VIII, Addison-Wesley, 1990, pp. 137 – 148. [6] a) M. J. Buerger, V. Venkatakrishnan, Proc. Natl. Acad. Sci. USA 1974, 71, 4348 – 4351; b) S. E. Lister, I. R. Evans, J. A. K. Howard, A. Coelho, J. S. O. Evans, Chem. Commun. 2004, 2540 – 2541; c) S. E. Lister, I. R. Evans, J. S. O. Evans, Inorg. Chem. 2009, 48, 9271 – 9281; d) L. Bindi, F. Nestola, A. Guastoni, L. Secco, Mineral. Mag. 2010, 74, 999 – 1012; e) C. Hoch, A. Simon, Angew. Chem. 2012, 124, 3316 – 3319; Angew. Chem. Int. Ed. 2012, 51, 3262 – 3265. [7] J. K. Burdett, C. Marians, J. F. Mitchell, Inorg. Chem. 1994, 33, 1848 – 1856. [8] L. Pauling, J. Am. Chem. Soc. 1929, 51, 1010 – 1026. [9] F. C. Hawthorne in Landmark Papers: Structure Topology (Ed.: F. C. Hawthorne), The Mineralogical Society of Great Britain and Ireland, Twickenham, 2006, p. L12. [10] W. H. Baur, E. T. Tillmanns, W. Hofmeister, Acta Crystallogr. Sect. B 1983, 39, 669 – 674. [11] A. L. Mackay, J. Klinowski, Comp. Math. Appl. Part B 1986, 12, 803 – 824. [12] A. L. Mackay, Crystallogr. Rep. 2001, 46, 524 – 526. [13] E. Estevez-Rams, R. Gonzlez-Frez, Z. Kristallogr. 2009, 224, 179 – 184. [14] W. Steurer, Acta Crystallogr. Sect. A 2011, A67, C184. [15] a) N. Rashevsky, Bull. Math. Biophys. 1955, 17, 229 – 235; b) E. Trucco, Bull. Math. Biophys. 1956, 18, 129 – 135; c) D. Bonchev,

Angew. Chem. Int. Ed. 2014, 53, 654 – 661

[25]

[26] [27] [28]

[29]

[30] [31] [32] [33]

[34] [35] [36] [37] [38] [39]

[40] [41]

SAR QSAR Environ. Res. 2003, 14, 199 – 214; d) M. Dehmer, A. Mowshowitz, Inform. Sci. 2011, 181, 57 – 78. a) S. V. Krivovichev, Acta Crystallogr. Sect. A 2012, 68, 393 – 398; b) S. V. Krivovichev, Struct. Chem. 2012, 23, 1045 – 1052; c) S. V. Krivovichev, Microporous Mesoporous Mater. 2013, 171, 223 – 229; d) S. V. Krivovichev, Miner. Mag. 2013, 77, 275 – 326. T. J. R. Weakley, E. R. Ylvisaker, R. J. Yager, J. E. Stephens, R. D. Wiegel, M. Mengis, P. Wu, P. Photinos, S. C. Abrahams, Acta Crystallogr. Sect. B 2004, 60, 705 – 715. S. V. Krivovichev, E. V. Kir’yanova, S. K. Filatov, P. C. Burns, Acta Crystallogr. Sect. C 2000, 56, 629 – 630. G.-C. Guo, W.-D. Cheng, J.-T. Chen, H.-H. Zhuang, J.-S. Huang, Q.-E. Zhang, Acta Crystallogr. Sect. C 1995, 51, 2469 – 2471. A. K. Pant, Acta Crystallogr. Sect. B 1968, 24, 1077 – 1083. P. J. Mohr, B. N. Taylor, D. B. Newell, Rev. Mod. Phys. 2008, 80, 633 – 730. Inorganic Crystal Structure Database. FIZ Karlsruhe GmbH 2012. V. A. Blatov, A. P. Shevchenko, V. N. Serezhkin, J. Appl. Crystallogr. 2000, 33, 1193. T. Weber, J. Dshemuchadse, M. Kobas, M. Conrad, B. Harbrecht, W. Steurer, Acta Crystallogr. Sect. B 2009, 65, 318 – 325. T. Mitra, P. Mir, A.-R. Tomsa, A. Merca, H. Bçgge, J. B. valos, J. M. Poblet, C. Bo, A. M ller, Chem. Eur. J. 2009, 15, 1844 – 1852. A. M ller, P. Gouzerh, Chem. Soc. Rev. 2012, 41, 7431 – 7463. a) P. C. Burns, Miner. Mag. 2011, 75, 1 – 25; b) J. Qiu, P. C. Burns, Chem. Rev. 2013, 113, 1097 – 1120. a) T. Z. Forbes, J. G. McAlpin, R. Murphy, P. C. Burns, Angew. Chem. 2008, 120, 2866 – 2869; Angew. Chem. Int. Ed. 2008, 47, 2824 – 2827; b) G. E. Sigmon, D. K. Unruh, J. Ling, B. Weaver, M. Ward, L. Pressprich, A. Simonetti, P. C. Burns, Angew. Chem. 2009, 121, 2775 – 2778; Angew. Chem. Int. Ed. 2009, 48, 2737 – 2740; c) J. Ling, C. M. Wallace, J. E. S. Szymanowski, P. C. Burns, Angew. Chem. 2010, 122, 7429 – 7431; Angew. Chem. Int. Ed. 2010, 49, 7271 – 7273. C. A. Ohlin, E. M. Villa, J. C. Fettinger, W. H. Casey, Angew. Chem. 2008, 120, 5716 – 5718; Angew. Chem. Int. Ed. 2008, 47, 5634 – 5636. B. S. Guiton, H. Wu, P. K. Davies, Chem. Mater. 2008, 20, 2860 – 2862. G. Costentin, A. Leclaire, M. M. Borel, A. Grandin, B. Raveau, Z. Kristallogr. 1992, 201, 53 – 58. E. K. Gordon, S. Samson, W. B. Kamb, Science 1966, 154, 1004 – 1007. A. Depla, E. Verheyen, A. Veyfeyken, M. Van Houteghem, K. Houthoofd, V. Van Speybroeck, M. Waroquier, C. E. A. Kirschhock, J. A. Martens, J. Phys. Chem. C 2011, 115, 11077 – 11088. C. Baerlocher, L. B. McCusker, D. H. Olson, Atlas of Zeolite Framework Types, 6th ed., Elsevier, Amsterdam, 2007. C. Baerlocher, T. Weber, L. B. McCusker, L. Palatinus, S. I. Zones, Science 2011, 333, 1134 – 1137. G. Nowogrocki, N. Penin, M. Touboul, Solid State Sci. 2003, 5, 795 – 803. A. M. Il’yinets, Yu. A. Malinovskii, Dokl. Akad. Nauk SSSR 1985, 282, 890 – 894. S. V. Krivovichev, O. Mentre, O. I. Siidra, M. Colmont, S. K. Filatov, Chem. Rev. 2013, 113, 6459 – 6535. a) G. Ferraris, E. Mackovicky, S. Merlino, Crystallography of Modular Materials, Oxford University Press, Oxford, 2004; b) M. G. Kanatzidis, Acc. Chem. Res. 2005, 38, 359 – 368. J. R. Goldsmith, J. Geol. 1953, 61, 439 – 451. a) R. Landauer, Phys. Lett. A 1996, 217, 188 – 193; b) A. Brut, A. Arakelyan, A. Petrosyan, S. Ciliberto, R. Dillenschneider, E. Lutz, Nature 2012, 483, 187 – 190.

2014 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim

www.angewandte.org

661